n^{-3}l^{-2}$. Hence, $6p$ elements such as Pb and Bi have a higher SOC strength as compared to that of the $3d$ or $5d$ elements studied before. Further tuning of SOC can be achieved by reducing the high rotational symmetry of single atom, [[i.e.,]{}]{} by using dimers of these elements. The effect of strong SOC on unsupported $6p$ dimers has been discussed recently [@Borisova2016a]. In an experimental and theoretical study, Schöneberg [[*et al.*]{}]{} [@Schoneberg2018] have achieved TAMR values of $\approx$ 20% by using suitably oriented Pb dimers on the Fe bilayer on W(110) substrate where magnetic domains with out-of-plane magnetization and domain walls with in-plane magnetization can be observed [@Bode2002].

In recent years noncollinear magnetic structures at transition-metal interfaces have gained popularity as promising candidates for spintronic applications due to their interesting dynamical and transport properties [@Fert2013; @Nagaosa2013]. A monolayer Mn grown on W(110) surface (Mn/W(110)) is a prominent example which exhibits a noncollinear magnetic structure with a cycloidal 173$^{\circ}$ spin-spiral ground state along the $[1\overline{1}0]$ direction [@Bode2007] that is driven by the Dzyaloshinskii-Moriya interaction. Using this magnetic surface with a noncollinear spin structure, it is possible to control the spin direction of adsorbed Co adatoms due to local exchange coupling which has been demonstrated in recent experiments using scanning tunneling microscopy (STM) by Serrate [[*et al.*]{}]{} [@Serrate2010; @Serrate2016]. The noncollinear spin state of the Mn monolayer is reflected due to hybridization even in the orbitals of the adsorbed Co adatom [@Haldar2018]. The possibility of controlling the magnetization direction of an adatom on this surface without the presence of external magnetic field makes this system very promising for TAMR studies. Compared to the domain walls of Fe/W(110) used in previous studies [@Schoneberg2018] the spin structure of this surface is known on the atomic scale and allows a quasi continuous rotation of the local spin quantization axis. Recently, Caffrey [[*et al.*]{}]{} have predicted TAMR values up to 50% for Ir adatoms, i.e
n^{-3}l^{-2}$. Hence, $ 6p$ elements such as Pb and Bi have a higher SOC strength as compare to that of the $ 3d$ or $ 5d$ chemical element studied before. Further tuning of SOC can be achieved by reduce the high rotational symmetry of individual atom, [ [ i.e., ] { } ] { } by using dimers of these component. The effect of strong SOC on unsupported $ 6p$ dimer has been discussed recently   [ @Borisova2016a ]. In an experimental and theoretical study, Schöneberg [ [ * et al. * ] { } ] { }   [ @Schoneberg2018 ] have achieved TAMR values of $ \approx$ 20% by use suitably orient Pb dimers on the Fe bilayer on W(110) substrate where magnetic sphere with out - of - plane magnetization and domain walls with in - airplane magnetization can be observed   [ @Bode2002 ]. 

 In recent year noncollinear magnetic structure at transition - metal interfaces have gained popularity as promising campaigner for spintronic applications due to their interesting dynamical and transport properties   [ @Fert2013; @Nagaosa2013 ]. A monolayer Mn grown on W(110) surface (Mn / W(110) ) is a prominent example which exhibits a noncollinear magnetic structure with a cycloidal 173$^{\circ}$ spin - spiral ground state along the $ [ 1\overline{1}0]$ direction   [ @Bode2007 ] that is drive by the Dzyaloshinskii - Moriya interaction. Using this magnetic surface with a noncollinear tailspin social organization, it is possible to control the spin direction of adsorbed Co adatoms due to local exchange coupling which has been demonstrated in recent experiment using scanning tunneling microscopy (STM) by Serrate [ [ * et al. * ] { } ] { }   [ @Serrate2010; @Serrate2016 ]. The noncollinear spin state of the Mn monolayer is reflected due to hybridization even in the orbitals of the adsorbed Co adatom   [ @Haldar2018 ]. The possibility of control the magnetization direction of an adatom on this surface without the presence of external magnetic discipline reach this system very promising for TAMR studies. Compared to the domain wall of Fe / W(110) used in previous studies   [ @Schoneberg2018 ] the tailspin structure of this airfoil is known on the atomic plate and allows a quasi continuous rotation of the local spin quantization axis. Recently, Caffrey [ [ * et al. * ] { } ] { } have predicted TAMR values up to 50% for Ir adatoms, i.e
n^{-3}l^{-2}$. Jence, $6p$ elements such as Pb and Bi have a highxr SOC atrength as compared to that of the $3v$ or $5d$ eltients studied befofe. Furtheg tuning if SIX can be argieved nv redhging chx high rotationsl symmetrf of single atmm, [[i.z.,]{}]{} by using dimers of these elements. Ehe effrch of strong SOS on tnsuliovted $6p$ dimers has been discussed recentny [@Borisova2016a]. Im an experimental and theogetifal study, Schöneberh [[*et al.*]{}]{} [@Schobebewt2018] have achiexed TAMR values of $\apptox$ 20% by using suitably oriented Ob dikers on thg Re tilayer on X(110) subsnrate where magnetic gomains with out-of-plake majnetuzation and domain wanls with in-plane mwgnetizathou can be observed [@Bode2002].

Un recett yaars bonzolmiiead magnftir structurea at transirion-metal interfacex rqve gained polulariey as promising candidates for spintronic apllications due to their interesting dynamicap and tragsport properties [@Fert2013; @Nagaosa2013]. A monolayer Mn growt on X(110) ruryqce (Mv/Q(110)) ls a prominent example which exhibits a noncojmimesr magnetic stvucture with a cyckoldsj 173$^{\circ}$ spin-spkral gxkuhd state along the $[1\overlige{1}0]$ dieection [@Boqe2007] tnat is driven by the Dzyalowhinskii-Morija ibteraction. Using tkis magnetic surgace eith a noncollinear spiu strudture, it is possible go control the soin dhrection of adsorbed Co adwtoms due to kocal ebchamge cotpling whifh has been demonstrated in rgcent axperimentd using scanning tunneling microscopy (STM) by Xesrane [[*et al.*]{}]{} [@Szrrate2010; @Serrate2016]. The goncollinear skin state of tfe Mn monomayer iv reflected due to hybriglzation even in the jrbirals of the xdsorbed Co adstom [@Haldag2018]. Uhe possibulity of controllikg thg jagnetization dnxextion of an adayom on tjix fgrface withogt tfe otesenze of exterkal magmetic field makes thhs sgstem very promisimg for TAMT studies. Compared to yhe domain walls ov Fe/W(110) usxd in lredious studies [@Schoneberg2018] the spjn structkre of this sursace is known on the atomic scale and allows a quasi coitinuous rotation of thw local spin quantieatlon axis. Recxntly, Saffrey [[*ed al.*]{}]{} have predicted RAMR values up to 50% for Ir adatoms, i.e
n^{-3}l^{-2}$. Hence, $6p$ elements such as Pb have higher SOC as compared to $5d$ studied before. Further of SOC can achieved by reducing the high rotational of single atom, [[i.e.,]{}]{} by using dimers of these elements. The effect of SOC on unsupported $6p$ dimers has been discussed recently [@Borisova2016a]. In an experimental theoretical Schöneberg al.*]{}]{} have achieved TAMR values of $\approx$ 20% by using suitably oriented Pb dimers on the Fe on W(110) substrate where magnetic domains with out-of-plane and domain walls with magnetization can be observed [@Bode2002]. recent noncollinear magnetic at interfaces gained popularity as candidates for spintronic applications due to their interesting dynamical and transport properties [@Fert2013; @Nagaosa2013]. A monolayer Mn on W(110) is a example exhibits noncollinear magnetic structure cycloidal 173$^{\circ}$ spin-spiral ground state along [@Bode2007] that is driven by the Dzyaloshinskii-Moriya interaction. this magnetic with a noncollinear spin structure, it possible to control the spin direction of adsorbed adatoms due to local exchange coupling which has been demonstrated in recent experiments using scanning (STM) by Serrate [[*et [@Serrate2010; @Serrate2016]. The spin of Mn is reflected to hybridization even in the orbitals of the adsorbed Co adatom The possibility of controlling the magnetization direction of an adatom surface the presence of magnetic field makes this very for TAMR studies. Compared domain of previous [@Schoneberg2018] spin structure of this is known on the atomic and allows a quasi spin quantization axis. Recently, Caffrey [[*et al.*]{}]{} have TAMR values up to 50% for Ir i.e
n^{-3}l^{-2}$. Hence, $6p$ elements such as Pb aNd Bi have a hIgher sOC StrEnGth aS comPared to that of tHE $3d$ or $5D$ elements studied before. furthEr TUninG Of sOC caN be achiEVeD BY reDuCiNg tHe HIgH rotaTioNal symmEtry of singLe aToM, [[i.e.,]{}]{} by using diMErS of these elEmeNts. The effect Of sTrong SoC On uNSuppoRteD $6p$ dimErs has BEen disCussed recEnTLy [@BoriSOva2016a]. In aN EXpErimEntal and theoreticAL sTUdy, Schöneberg [[*eT al.*]{}]{} [@SchOnEBeRG2018] HavE acHieved TAMR VaLues oF $\Approx$ 20% bY UsING SuiTAbly oriented PB dimers on thE fe bIlayer On w(110) suBStrate Where MaGNetIc domains wiTh ouT-of-plane mAgnetiZAtion anD Domain wAlls wiTh iN-plAne mAGnEtIzaTiON caN Be ObsERveD [@Bode2002].

In rEcEnT yearS nonCOLLIneaR maGnetIc strUctures at tranSitIon-mETal InterFaces Have GaIned pOpularIty as PrOmising candidatEs foR spintronIc aPpLicAtIons dUE to theIr iNteResting DynamicAL anD tRANSpOrt properties [@Fert2013; @NAgAOSa2013]. a monolayEr Mn grOWn On w(110) Surface (MN/W(110)) Is a PromINEnt exAmplE WhIch exhibIts a noNCoLlInear maGnEtic stRuCtuRe wIth a cYCloiDal 173$^{\cirC}$ spin-spiRal grOUnd state along tHE $[1\overline{1}0]$ direCTiON [@boDE2007] thaT is Driven by the dzyaLOshiNskiI-moRiyA InterActioN. USInG This magnetic surface WiTh a nonColliNear spin strucTure, it is poSSIBle to conTrol THe SPin direction of AdsorBed Co adatoMS due to loCal exChange coUpling whiCH Has been dEmoNstRatEd iN REcEnt experimentS USing ScAnning tUnnEling miCroScoPy (StM) bY SErrate [[*et aL.*]{}]{} [@Serrate2010; @seRrAtE2016]. THe nOncolLInear spiN sTatE oF thE Mn moNOlayer Is refLectEd DuE To hYbridizATiON Even In ThE orbItaLs Of the AdsoRBed co adatoM [@Haldar2018]. ThE poSSibiLiTy Of contrOlling the magnEtIzation dirEcTioN of an aDATom on thiS surface without the preseNCe of extErnAl magNetiC field makEs tHis sysTem VEry proMising For TAmR StuDIEs. ComPAReD to ThE domain walLS Of FE/W(110) useD iN preVious stUdies [@Schoneberg2018] the SPin Structure of thIs sUrfaCE Is KnoWN oN The AtOMic SCAle and allows a quAsi continuOuS RoTation of thE LocAl Spin quaNtizatiOn axiS. recentlY, Caffrey [[*eT al.*]{}]{} have prEdIcteD taMR Values up to 50% For Ir adaToms, i.e
n^{-3}l^{-2}$. Hence, $6p$  elementssuchasPban d Bi  hav e a higher SOC stre ngth as compared to th at of  t h e $3 d $or $5 d$ elem e nt s stu di ed  be fo r e.  Furt her  tuning  of SOC ca n b eachieved byr ed ucing thehig h rotational  sy mmetry  o f s i ngleato m, [[ i.e.,] { }]{} b y using d im e rs oft hese el e m en ts.The effect of str o ng SOC on unsuppo rted $ 6p $  d i m ers  ha s been dis cu ssedr ecently [@ B o r iso v a2016a]. In a n experimen t aland th eo ret i cal st udy,Sc h öne berg [[*etal.* ]{}]{} [@ Schone b erg2018 ]  have a chieve d T AMR  val u es  o f $ \a p pro x $20% byusing su it ab ly or ient e d P b di mer s on  theFe bilayer on  W( 110) sub strat e whe re m ag netic  domai ns wi th  out-of-plane m agne tizationand  d oma in  wall s  within- pla ne magn etizati o n c an b e  o bserved [@Bode2002 ]. In  recentyearsn on co l linear m ag net ic s t r uctur es a t  t ransitio n-meta l  i nt erfaces  h ave ga in edpop ulari t y as  promi sing can didat e s for spintron i c application s  d u e  t o  the irinteresting  dyn a mica l an d  t ran s portprope rt i es [@Fert2013; @Nagaos a2 013].A mon olayer Mn gro wn on W(11 0 ) surface(Mn/ W (1 1 0)) is a promi nentexample wh i ch exhib its a  noncoll inear mag n e tic stru ctu rewit h a c yc loidal 173$^{ \ c irc} $spin-sp ira l groun d s tat e a lon gthe $[1\o verline{ 1} 0] $di rec tion[ @Bode200 7]  th at  is  driv e n by t he Dz yalo sh in s kii -Moriya in t e ract io n.  Usi ngth is ma gnet i c s urfacewith a no nco l line ar  s pin str ucture, it is  p ossible to  c ont rol th e spin dir ection of adsorbed Co a d atoms d ueto lo calexchangecou plingwhi c h hasbeen d emons tr ate d in re c e nt  ex pe riments us i n g s canni ng  tun nelingmicroscopy (STM) b y  Se rrate [[*et a l.* ]{}] { }  [ @Se r ra t e20 10 ;  @S e r rate2016]. Thenoncolline ar sp in state o f  th eMn mono layer i s ref l ected d ue to hyb ridizatio neven i n t he orbital s of the  adsorbed Co ad a to m [@H ald ar2018 ].  Th e pos sibili t y o f con trolli ng  the m agnet iz ation di rection of an adatom on  thissurfa cewithout t hep res ence of e xter nal magnet icfie ld ma kes thissyst e mver y  prom isin g  for TAMR st udi e s .Compared to t h e d omain  wa l ls ofFe/W (110) used in pre v ious studies [ @Sch o n ebe rg2 0 18]th e spin structu reof t his surf ac e is knownon the a to m ic sc ale an d allo ws a qu a s ic ontinu ousrot ation ofthe  l o cal spi nqu a ntizat ionax is. Re cently ,  Caf f r ey [[*et al.*]{} ]{} h a v e pre d ict ed TA MR  values up t o 50% forIr adatoms,  i.e
n^{-3}l^{-2}$. Hence,_$6p$ elements_such as Pb and_Bi have_a_higher SOC_strength_as compared to_that of the_$3d$ or $5d$ elements_studied before. Further_tuning_of SOC can be achieved by reducing the high rotational symmetry of single atom,_[[i.e.,]{}]{}_by using_dimers_of_these elements. The effect of_strong SOC on unsupported $6p$_dimers has_been discussed recently [@Borisova2016a]. In an experimental and theoretical_study,_Schöneberg [[*et al.*]{}]{} [@Schoneberg2018]_have achieved TAMR values of $\approx$ 20% by using_suitably oriented Pb dimers on the_Fe bilayer on_W(110)_substrate_where magnetic domains with_out-of-plane magnetization and domain walls with_in-plane magnetization can be observed [@Bode2002].

In recent_years noncollinear magnetic structures at transition-metal interfaces_have gained popularity as promising candidates_for spintronic applications due to_their interesting_dynamical and transport properties [@Fert2013; @Nagaosa2013]._A monolayer Mn_grown on_W(110) surface (Mn/W(110))_is a prominent example which exhibits_a noncollinear magnetic_structure with a cycloidal 173$^{\circ}$ spin-spiral_ground_state along the_$[1\overline{1}0]$_direction [@Bode2007]_that is_driven by the_Dzyaloshinskii-Moriya_interaction. Using_this_magnetic surface with a noncollinear spin_structure,_it is possible to control the spin_direction of adsorbed Co_adatoms_due to local exchange_coupling which has been demonstrated_in recent experiments using scanning tunneling_microscopy (STM)_by Serrate_[[*et al.*]{}]{} [@Serrate2010; @Serrate2016]. The noncollinear spin state of the Mn monolayer_is reflected due to hybridization even_in the orbitals of_the adsorbed_Co_adatom [@Haldar2018]. The possibility_of_controlling the_magnetization direction of an adatom on this_surface without_the presence of external magnetic field_makes this system very_promising_for TAMR studies. Compared to the_domain walls of Fe/W(110) used in_previous studies [@Schoneberg2018] the spin structure_of_this_surface is known on the_atomic scale and allows a quasi_continuous rotation of_the local spin quantization axis. Recently, Caffrey_[[*et_al.*]{}]{} have predicted TAMR values up_to_50% for Ir adatoms, i.e